viii CONTENTS Further Reading 95 Problems 95 4 Fluid Flow and Metal Evaporation in Welding 97 4.1 Fluid Flow in Arcs 97 4.2 Fluid Flow in Weld Pools 103 4.3 Metal Evaporation 114 4.4 Active Flux GTAW 116 References 117 Further Reading 119 Problems 120 5 Residual Stresses, Distortion, and Fatigue 122 5.1 Residual Stresses 122 5.2 Distortion 126 5.3 Fatigue 131 5.4 Case Studies 137 References 140 Further Reading 141 Problems 141II THE FUSION ZONE 143 6 Basic Solidiﬁcation Concepts 145 6.1 Solute Redistribution during Solidiﬁcation 145 6.2 Solidiﬁcation Modes and Constitutional Supercooling 155 6.3 Microsegregation and Banding 160 6.4 Effect of Cooling Rate 163 6.5 Solidiﬁcation Path 166 References 167 Further Reading 168 Problems 169 7 Weld Metal Solidiﬁcation I: Grain Structure 170 7.1 Epitaxial Growth at Fusion Boundary 170 7.2 Nonepitaxial Growth at Fusion Boundary 172 7.3 Competitive Growth in Bulk Fusion Zone 174 7.4 Effect of Welding Parameters on Grain Structure 174 7.5 Weld Metal Nucleation Mechanisms 178 7.6 Grain Structure Control 187
CONTENTS ix References 195 Further Reading 197 Problems 197 8 Weld Metal Solidiﬁcation II: Microstructure within Grains 199 8.1 Solidiﬁcation Modes 199 8.2 Dendrite and Cell Spacing 204 8.3 Effect of Welding Parameters 206 8.4 Reﬁning Microstructure within Grains 209 References 213 Further Reading 213 Problems 214 9 Post-Solidiﬁcation Phase Transformations 216 9.1 Ferrite-to-Austenite Transformation in Austenitic Stainless Steel Welds 216 9.2 Austenite-to-Ferrite Transformation in Low-Carbon, Low-Alloy Steel Welds 232 References 239 Further Reading 241 Problems 24110 Weld Metal Chemical Inhomogeneities 243 10.1 Microsegregation 243 10.2 Banding 249 10.3 Inclusions and Gas Porosity 250 10.4 Inhomogeneities Near Fusion Boundary 252 10.5 Macrosegregation in Bulk Weld Metal 255 References 260 Further Reading 261 Problems 26111 Weld Metal Solidiﬁcation Cracking 263 11.1 Characteristics, Cause, and Testing 263 11.2 Metallurgical Factors 268 11.3 Mechanical Factors 284 11.4 Reducing Solidiﬁcation Cracking 285 11.5 Case Study: Failure of a Large Exhaust Fan 295 References 296 Further Reading 299 Problems 299
x CONTENTSIII THE PARTIALLY MELTED ZONE 301 12 Formation of the Partially Melted Zone 303 12.1 Evidence of Liquation 303 12.2 Liquation Mechanisms 304 12.3 Directional Solidiﬁcation of Liquated Material 314 12.4 Grain Boundary Segregation 314 12.5 Grain Boundary Solidiﬁcation Modes 316 12.6 Partially Melted Zone in Cast Irons 318 References 318 Problems 319 13 Difﬁculties Associated with the Partially Melted Zone 321 13.1 Liquation Cracking 321 13.2 Loss of Strength and Ductility 328 13.3 Hydrogen Cracking 328 13.4 Remedies 330 References 336 Problems 338IV THE HEAT-AFFECTED ZONE 341 14 Work-Hardened Materials 343 14.1 Background 343 14.2 Recrystallization and Grain Growth in Welding 347 14.3 Effect of Welding Parameters and Process 349 References 351 Further Reading 352 Problems 352 15 Precipitation-Hardening Materials I: Aluminum Alloys 353 15.1 Background 353 15.2 Al–Cu–Mg and Al–Mg–Si Alloys 359 15.3 Al–Zn–Mg Alloys 367 15.4 Friction Stir Welding of Aluminum Alloys 370 References 371 Further Reading 372 Problems 372 16 Precipitation-Hardening Materials II: Nickel-Base Alloys 375 16.1 Background 375
CONTENTS xi 16.2 Reversion of Precipitate and Loss of Strength 379 16.3 Postweld Heat Treatment Cracking 384 References 390 Further Reading 392 Problems 39217 Transformation-Hardening Materials: Carbon and Alloy Steels 393 17.1 Phase Diagram and CCT Diagrams 393 17.2 Carbon Steels 396 17.3 Low-Alloy Steels 404 17.4 Hydrogen Cracking 410 17.5 Reheat Cracking 418 17.6 Lamellar Tearing 422 17.7 Case Studies 425 References 427 Further Reading 429 Problems 43018 Corrosion-Resistant Materials: Stainless Steels 431 18.1 Classiﬁcation of Stainless Steels 431 18.2 Austenitic Stainless Steels 433 18.3 Ferritic Stainless Steels 446 18.4 Martensitic Stainless Steels 449 18.5 Case Study: Failure of a Pipe 451 References 452 Further Reading 453 Problems 454Index 455
PREFACESince the publication of the ﬁrst edition of this book in 1987, there has beenmuch new progress made in welding metallurgy. The purpose for the secondedition is to update and improve the ﬁrst edition. Examples of improvementsinclude (1) much sharper photomicrographs and line drawings; (2) integrationof the phase diagram, thermal cycles, and kinetics with the microstructure toexplain microstructural development and defect formation in welds; and (3)additional exercise problems. Speciﬁc revisions are as follows. In Chapter 1 the illustrations for all welding processes have been re-drawn to show both the overall process and the welding area. In Chapter2 the heat source efﬁciency has been updated and the melting efﬁciencyadded. Chapter 3 has been revised extensively, with the dissolution ofatomic nitrogen, oxygen, and hydrogen in the molten metal considered andelectrochemical reactions added. Chapter 4 has also been revised extensively,with the arc added, and with ﬂow visualization, arc plasma dragging, andturbulence included in weld pool convection. Shot peening is added toChapter 5. Chapter 6 has been revised extensively, with solute redistribution andmicrosegregation expanded and the solidiﬁcation path added. Chapter 7 nowincludes nonepitaxial growth at the fusion boundary and formation of non-dendritic equiaxed grains. In Chapter 8 solidiﬁcation modes are explained withmore illustrations. Chapter 9 has been expanded signiﬁcantly to add ferriteformation mechanisms, new ferrite prediction methods, the effect of coolingrate, and factors affecting the austenite–ferrite transformation. Chapter 10now includes the effect of both solid-state diffusion and dendrite tip under-cooling on microsegregation. Chapter 11 has been revised extensively toinclude the effect of eutectic reactions, liquid distribution, and ductility ofthe solidifying metal on solidiﬁcation cracking and the calculation of fractionof liquid in multicomponent alloys. Chapter 12 has been rewritten completely to include six different liquationmechanisms in the partially melted zone (PMZ), the direction and modes ofgrain boundary (GB) solidiﬁcation, and the resultant GB segregation. Chapter13 has been revised extensively to include the mechanism of PMZ crackingand the effect of the weld-metal composition on cracking. Chapter 15 now includes the heat-affected zone (HAZ) in aluminum–lithium–copper welds and friction stir welds and Chapter 16 the HAZ ofInconel 718. Chapter 17 now includes the effect of multiple-pass welding on xiii
xiv PREFACEreheat cracking and Chapter 18 the grain boundary chromium depletion in asensitized austenitic stainless steel. The author thanks the National Science Foundation and NASA forsupporting his welding research, from which this book draws frequently.He also thanks the American Welding Society and ASM International for per-missions to use numerous copyrighted materials. Finally, he thanks C. Huang,G. Cao, C. Limmaneevichitr, H. D. Lu, K. W. Keehn, and T. Tantanawat for pro-viding technical material, requesting permissions, and proofreading. Sindo KouMadison, Wisconsin
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-4PART IIntroduction
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-41 Fusion Welding ProcessesFusion welding processes will be described in this chapter, including gaswelding, arc welding, and high-energy beam welding. The advantages and dis-advantages of each process will be discussed.1.1 OVERVIEW1.1.1 Fusion Welding ProcessesFusion welding is a joining process that uses fusion of the base metal to makethe weld. The three major types of fusion welding processes are as follows: 1. Gas welding: Oxyacetylene welding (OAW) 2. Arc welding: Shielded metal arc welding (SMAW) Gas–tungsten arc welding (GTAW) Plasma arc welding (PAW) Gas–metal arc welding (GMAW) Flux-cored arc welding (FCAW) Submerged arc welding (SAW) Electroslag welding (ESW) 3. High-energy beam welding: Electron beam welding (EBW) Laser beam welding (LBW) Since there is no arc involved in the electroslag welding process, it is notexactly an arc welding process. For convenience of discussion, it is groupedwith arc welding processes.1.1.2 Power Density of Heat SourceConsider directing a 1.5-kW hair drier very closely to a 304 stainless steel sheet1.6 mm (1/16 in.) thick. Obviously, the power spreads out over an area of roughly 3
4 FUSION WELDING PROCESSES50 mm (2 in.) diameter, and the sheet just heats up gradually but will not melt.With GTAW at 1.5 kW, however, the arc concentrates on a small area of about6 mm (1/4 in.) diameter and can easily produce a weld pool. This example clearlydemonstrates the importance of the power density of the heat source inwelding. The heat sources for the gas, arc, and high-energy beam welding processesare a gas ﬂame, an electric arc, and a high-energy beam, respectively. Thepower density increases from a gas ﬂame to an electric arc and a high-energybeam. As shown in Figure 1.1, as the power density of the heat sourceincreases, the heat input to the workpiece that is required for weldingdecreases. The portion of the workpiece material exposed to a gas ﬂame heatsup so slowly that, before any melting occurs, a large amount of heat is alreadyconducted away into the bulk of the workpiece. Excessive heating can causedamage to the workpiece, including weakening and distortion. On the con-trary, the same material exposed to a sharply focused electron or laser beamcan melt or even vaporize to form a deep keyhole instantaneously, and beforemuch heat is conducted away into the bulk of the workpiece, welding is com-pleted (1). Therefore, the advantages of increasing the power density of the heatsource are deeper weld penetration, higher welding speeds, and better weldquality with less damage to the workpiece, as indicated in Figure 1.1. Figure1.2 shows that the weld strength (of aluminum alloys) increases as the heatinput per unit length of the weld per unit thickness of the workpiece decreases(2). Figure 1.3a shows that angular distortion is much smaller in EBW than in Increasing damage to workpiece Heat input to workpiece gas welding arc welding Increasing penetration, welding speed, weld quality, high energy equipment cost beam welding Power density of heat sourceFigure 1.1 Variation of heat input to the workpiece with power density of the heatsource.
OVERVIEW 5 60 2219 Strength, ksi 50 5083 7039 40 30 6061 5 10 50 100 500 Heat input, kJ/in./in.Figure 1.2 Variation of weld strength with heat input per unit length of weld per unitthickness of workpiece. Reprinted from Mendez and Eagar (2). 8 Productivity, inch of weld/s 0.04 0.4 4 40 400 7 Distortion angle α degree 107 10 6 Laser Capital equipment, dollars Power density, W/m 2 electron beam t 4 105 105 W α GTA 2 Arc 103 103 EBW Flame 0 0 20 40 0.1 1 10 100 (a) Weld thickness t, mm (b) Productivity, cm/sFigure 1.3 Comparisons between welding processes: (a) angular distortion; (b) capitalequipment cost. Reprinted from Mendez and Eagar (2).GTAW (2). Unfortunately, as shown in Figure 1.3b, the costs of laser and elec-tron beam welding machines are very high (2).1.1.3 Welding Processes and MaterialsTable 1.1 summarizes the fusion welding processes recommended for carbonsteels, low-alloy steels, stainless steels, cast irons, nickel-base alloys, and
TABLE 1.1 Overview of Welding Processesa6 Material Thicknessb SMAW SAW GMAW FCAW GTAW PAW ESW OFW EBW LBW Carbon S ✕ ✕ ✕ ✕ ✕ ✕ ✕ steels I ✕ ✕ ✕ ✕ ✕ ✕ ✕ ✕ M ✕ ✕ ✕ ✕ ✕ ✕ ✕ T ✕ ✕ ✕ ✕ ✕ ✕ ✕ Low-alloy S ✕ ✕ ✕ ✕ ✕ ✕ ✕ steels I ✕ ✕ ✕ ✕ ✕ ✕ ✕ M ✕ ✕ ✕ ✕ ✕ ✕ T ✕ ✕ ✕ ✕ ✕ ✕ Stainless S ✕ ✕ ✕ ✕ ✕ ✕ ✕ ✕ steels I ✕ ✕ ✕ ✕ ✕ ✕ ✕ ✕ M ✕ ✕ ✕ ✕ ✕ ✕ ✕ T ✕ ✕ ✕ ✕ ✕ ✕ Cast iron I ✕ ✕ M ✕ ✕ ✕ ✕ ✕ T ✕ ✕ ✕ ✕ ✕ Nickel S ✕ ✕ ✕ ✕ ✕ ✕ ✕ and alloys I ✕ ✕ ✕ ✕ ✕ ✕ ✕ M ✕ ✕ ✕ ✕ ✕ ✕ T ✕ ✕ ✕ ✕ Aluminum S ✕ ✕ ✕ ✕ ✕ ✕ and alloys I ✕ ✕ ✕ ✕ M ✕ ✕ ✕ T ✕ ✕ a Process code: SMAW, shielded metal arc welding; SAW, submerged arc welding; GMAW, gas–metal arc welding; FCAW, ﬂux-cored arc welding; GTAW, gas–tungsten arc welding; PAW, plasma arc welding; ESW, electroslag welding; OFW, oxyfuel gas welding; EBW, electron beam welding; LBW, laser beam welding. b Abbreviations: S, sheet, up to 3 mm (1/8 in.); I, intermediate, 3–6 mm (1/8–1/4 in.); M, medium, 6–19 mm (1/4–3/4 in.); T, thick, 19 mm (3/4 in.) and up; X, recommended. Source: Welding Handbook (3).
OXYACETYLENE WELDING 7 (a) butt joint t (b) lap joint join ed ge (e) corner joint (c) T-joint (d) Figure 1.4 Five basic types of weld joint designs.aluminum alloys (3). For one example, GMAW can be used for all the materi-als of almost all thickness ranges while GTAW is mostly for thinner workpieces.For another example, any arc welding process that requires the use of a ﬂux,such as SMAW, SAW, FCAW, and ESW, is not applicable to aluminum alloys.1.1.4 Types of Joints and Welding PositionsFigure 1.4 shows the basic weld joint designs in fusion welding: the butt, lap,T-, edge, and corner joints. Figure 1.5 shows the transverse cross section ofsome typical weld joint variations. The surface of the weld is called the face,the two junctions between the face and the workpiece surface are called thetoes, and the portion of the weld beyond the workpiece surface is called thereinforcement. Figure 1.6 shows four welding positions.1.2 OXYACETYLENE WELDING1.2.1 The ProcessGas welding is a welding process that melts and joins metals by heating themwith a ﬂame caused by the reaction between a fuel gas and oxygen. Oxy-acetylene welding (OAW), shown in Figure 1.7, is the most commonly usedgas welding process because of its high ﬂame temperature. A ﬂux may be usedto deoxidize and cleanse the weld metal. The ﬂux melts, solidiﬁes, and formsa slag skin on the resultant weld metal. Figure 1.8 shows three different typesof ﬂames in oxyacetylene welding: neutral, reducing, and oxidizing (4), whichare described next.1.2.2 Three Types of FlamesA. Neutral Flame This refers to the case where oxygen (O2) and acetylene(C2H2) are mixed in equal amounts and burned at the tip of the welding torch.A short inner cone and a longer outer envelope characterize a neutral ﬂame
8 FUSION WELDING PROCESSES Reinforcement Toe (a) Toe (d) Toe Butt joint; T-joint; square weld fillet weld (b) Reinforcement (e) Toe Toe Toe Root Butt joint; T-joint; single-V-groove weld single bevel weld (c) Toe Toe Lap joint; fillet weld Figure 1.5 Typical weld joint variations.(Figure 1.8a). The inner cone is the area where the primary combustion takesplace through the chemical reaction between O2 and C2H2, as shown in Figure1.9. The heat of this reaction accounts for about two-thirds of the total heatgenerated. The products of the primary combustion, CO and H2, react with O2from the surrounding air and form CO2 and H2O. This is the secondary com-bustion, which accounts for about one-third of the total heat generated. Thearea where this secondary combustion takes place is called the outer enve-lope. It is also called the protection envelope since CO and H2 here consumethe O2 entering from the surrounding air, thereby protecting the weld metalfrom oxidation. For most metals, a neutral ﬂame is used.B. Reducing Flame When excess acetylene is used, the resulting ﬂame iscalled a reducing ﬂame.The combustion of acetylene is incomplete.As a result,a greenish acetylene feather between the inert cone and the outer envelopecharacterizes a reducing ﬂame (Figure 1.8b). This ﬂame is reducing in natureand is desirable for welding aluminum alloys because aluminum oxidizeseasily. It is also good for welding high-carbon steels (also called carburizingﬂame in this case) because excess oxygen can oxidize carbon and form CO gasporosity in the weld metal.
OXYACETYLENE WELDING 9 (a) flat (b) horizontal (c) vertical (d) overhead Figure 1.6 Four welding positions. Flow meter Regulator Oxygen Welding direction Valve O2 Gas torch C2H2 Acetylene (a) Workpiece Oxygen/acetylene mixture Filler rod Protection envelope Primary combustion Metal droplet Slag Weld (b) metal Base metal Weld poolFigure 1.7 Oxyacetylene welding: (a) overall process; (b) welding area enlarged.
10 FUSION WELDING PROCESSES Neutral Flame inner cone (a) inner cone Reducing Flame (b) acetylene feather inner cone Oxidizing Flame (c)Figure 1.8 Three types of ﬂames in oxyacetylene welding. Modiﬁed from WeldingJournal (4). Courtesy of American Welding Society. Gas C2H2 + O2 Primary combustion in inner cone (2/3 total heat) : Torch 2C2H2 + 2O2 (from cylinder) 4CO + 2H2 inner Secondary combustion in outer 2800 - 3500 oC cone envelope (1/3 total heat) : Flame 2500 oC outer 4CO + 2O2 (from air) 4CO2 envelope 2H2 + O2 (from air) 2H2O 1000 oCFigure 1.9 Chemical reactions and temperature distribution in a neutral oxyacetyleneﬂame.C. Oxidizing Flame When excess oxygen is used, the ﬂame becomes oxi-dizing because of the presence of unconsumed oxygen. A short white innercone characterizes an oxidizing ﬂame (Figure 1.8c). This ﬂame is preferredwhen welding brass because copper oxide covers the weld pool and thus pre-vents zinc from evaporating from the weld pool.1.2.3 Advantages and DisadvantagesThe main advantage of the oxyacetylene welding process is that the equip-ment is simple, portable, and inexpensive. Therefore, it is convenient for main-tenance and repair applications. However, due to its limited power density, the
SHIELDED METAL ARC WELDING 11welding speed is very low and the total heat input per unit length of the weldis rather high, resulting in large heat-affected zones and severe distortion. Theoxyacetylene welding process is not recommended for welding reactive metalssuch as titanium and zirconium because of its limited protection power.1.3 SHIELDED METAL ARC WELDING1.3.1 The ProcessShielded metal arc welding (SMAW) is a process that melts and joins metalsby heating them with an arc established between a sticklike covered electrodeand the metals, as shown in Figure 1.10. It is often called stick welding.The electrode holder is connected through a welding cable to one terminalof the power source and the workpiece is connected through a second cableto the other terminal of the power source (Figure 1.10a). The core of the covered electrode, the core wire, conducts the electriccurrent to the arc and provides ﬁller metal for the joint. For electrical contact,the top 1.5 cm of the core wire is bare and held by the electrode holder. Theelectrode holder is essentially a metal clamp with an electrically insulatedoutside shell for the welder to hold safely. The heat of the arc causes both the core wire and the ﬂux covering at theelectrode tip to melt off as droplets (Figure 1.10b). The molten metal collectsin the weld pool and solidiﬁes into the weld metal. The lighter molten ﬂux, onthe other hand, ﬂoats on the pool surface and solidiﬁes into a slag layer at thetop of the weld metal.1.3.2 Functions of Electrode CoveringThe covering of the electrode contains various chemicals and even metalpowder in order to perform one or more of the functions described below.A. Protection It provides a gaseous shield to protect the molten metal fromair. For a cellulose-type electrode, the covering contains cellulose, (C6H10O5)x.A large volume of gas mixture of H2, CO, H2O, and CO2 is produced whencellulose in the electrode covering is heated and decomposes. For a limestone-(CaCO3Ϫ) type electrode, on the other hand, CO2 gas and CaO slag form whenthe limestone decomposes. The limestone-type electrode is a low-hydrogen-type electrode because it produces a gaseous shield low in hydrogen. It is oftenused for welding metals that are susceptible to hydrogen cracking, such ashigh-strength steels.B. Deoxidation It provides deoxidizers and ﬂuxing agents to deoxidize andcleanse the weld metal. The solid slag formed also protects the already solid-iﬁed but still hot weld metal from oxidation.
12 FUSION WELDING PROCESSES (a) Electrode Power holder Source Welding Cable 1 direction Stick electrode Cable 2 Workpiece Core wire (b) Flux covering Metal Gaseous shield droplet Flux Arc droplet Slag Weld metal Base metal Weld poolFigure 1.10 Shielded metal arc welding: (a) overall process; (b) welding area enlarged.C. Arc Stabilization It provides arc stabilizers to help maintain a stablearc. The arc is an ionic gas (a plasma) that conducts the electric current.Arc stabilizers are compounds that decompose readily into ions in the arc,such as potassium oxalate and lithium carbonate. They increase the electricalconductivity of the arc and help the arc conduct the electric current moresmoothly.D. Metal Addition It provides alloying elements and/or metal powder tothe weld pool. The former helps control the composition of the weld metalwhile the latter helps increase the deposition rate.1.3.3 Advantages and DisadvantagesThe welding equipment is relatively simple, portable, and inexpensive as com-pared to other arc welding processes. For this reason, SMAW is often used formaintenance, repair, and ﬁeld construction. However, the gas shield in SMAWis not clean enough for reactive metals such as aluminum and titanium. Thedeposition rate is limited by the fact that the electrode covering tends to over-heat and fall off when excessively high welding currents are used. The limitedlength of the electrode (about 35 cm) requires electrode changing, and thisfurther reduces the overall production rate.
GAS–TUNGSTEN ARC WELDING 131.4 GAS–TUNGSTEN ARC WELDING1.4.1 The ProcessGas–tungsten arc welding (GTAW) is a process that melts and joins metals byheating them with an arc established between a nonconsumable tungsten elec-trode and the metals, as shown in Figure 1.11. The torch holding the tungstenelectrode is connected to a shielding gas cylinder as well as one terminal ofthe power source, as shown in Figure 1.11a. The tungsten electrode is usuallyin contact with a water-cooled copper tube, called the contact tube, as shownin Figure 1.11b, which is connected to the welding cable (cable 1) from theterminal. This allows both the welding current from the power source toenter the electrode and the electrode to be cooled to prevent overheating. Theworkpiece is connected to the other terminal of the power source through adifferent cable (cable 2). The shielding gas goes through the torch body andis directed by a nozzle toward the weld pool to protect it from the air. Pro-tection from the air is much better in GTAW than in SMAW because an inertgas such as argon or helium is usually used as the shielding gas and becausethe shielding gas is directed toward the weld pool. For this reason, GTAW is Flow Regulator meter (a) Welding Shielding gas direction Torch cylinder Cable 1 Filler rod Cable 2 Power source Workpiece Tungsten electrode Shielding (b) gas Contact tube Filler Cable 1 rod Shielding gas Shielding gas nozzle Metal Arc droplet Weld metal Base metal Weld poolFigure 1.11 Gas–tungsten arc welding: (a) overall process; (b) welding area enlarged.
14 FUSION WELDING PROCESSESalso called tungsten–inert gas (TIG) welding. However, in special occasions anoninert gas (Chapter 3) can be added in a small quantity to the shielding gas.Therefore, GTAW seems a more appropriate name for this welding process.When a ﬁller rod is needed, for instance, for joining thicker materials, it canbe fed either manually or automatically into the arc.1.4.2 PolarityFigure 1.12 shows three different polarities in GTAW (5), which are describednext.A. Direct-Current Electrode Negative (DCEN) This, also called the straightpolarity, is the most common polarity in GTAW. The electrode is connected tothe negative terminal of the power supply. As shown in Figure 1.12a, electronsare emitted from the tungsten electrode and accelerated while travelingthrough the arc. A signiﬁcant amount of energy, called the work function, isrequired for an electron to be emitted from the electrode. When the electronenters the workpiece, an amount of energy equivalent to the work function isreleased. This is why in GTAW with DCEN more power (about two-thirds) islocated at the work end of the arc and less (about one-third) at the electrodeend. Consequently, a relatively narrow and deep weld is produced.B. Direct-Current Electrode Positive (DCEP) This is also called the reversepolarity. The electrode is connected to the positive terminal of the powersource. As shown in Figure 1.12b, the heating effect of electrons is now at thetungsten electrode rather than at the workpiece. Consequently, a shallow weldis produced. Furthermore, a large-diameter, water-cooled electrodes must beused in order to prevent the electrode tip from melting. The positive ions ofthe shielding gas bombard the workpiece, as shown in Figure 1.13, knockingoff oxide ﬁlms and producing a clean weld surface. Therefore, DCEP can be DC electrode DC electrode AC negative positive pool deep weld, shallow weld, intermediate no surface cleaning surface cleaning (a) (b) (c) Figure 1.12 Three different polarities in GTAW.
GAS–TUNGSTEN ARC WELDING 15 Cleaning action (electrode positive) bombarding heavy ion Ar+ knocked-off atoms M O oxide film on surface M O M O M Workpiece (negative) Figure 1.13 Surface cleaning action in GTAW with DC electrode positive.used for welding thin sheets of strong oxide-forming materials such as alu-minum and magnesium, where deep penetration is not required.C. Alternating Current (AC) Reasonably good penetration and oxidecleaning action can both be obtained, as illustrated in Figure 1.12c.This is oftenused for welding aluminum alloys.1.4.3 ElectrodesTungsten electrodes with 2% cerium or thorium have better electronemissivity, current-carrying capacity, and resistance to contamination thanpure tungsten electrodes (3). As a result, arc starting is easier and the arc ismore stable. The electron emissivity refers to the ability of the electrode tipto emit electrons. A lower electron emissivity implies a higher electrode tiptemperature required to emit electrons and hence a greater risk of melting thetip.1.4.4 Shielding GasesBoth argon and helium can be used. Table 1.2 lists the properties of someshielding gases (6). As shown, the ionization potentials for argon and heliumare 15.7 and 24.5 eV (electron volts), respectively. Since it is easier to ionizeargon than helium, arc initiation is easier and the voltage drop across the arcis lower with argon. Also, since argon is heavier than helium, it offers moreeffective shielding and greater resistance to cross draft than helium. WithDCEP or AC, argon also has a greater oxide cleaning action than helium.These advantages plus the lower cost of argon make it more attractive forGTAW than helium.
16 FUSION WELDING PROCESSESTABLE 1.2 Properties of Shielding Gases Used for Welding Molecular Speciﬁc Gravity Ionization Chemical Weight with Respect to Air Density PotentialGas Symbol (g/mol) at 1 atm and 0°C (g/L) (eV)Argon Ar 39.95 1.38 1.784 15.7Carbon dioxide CO2 44.01 1.53 1.978 14.4Helium He 4.00 0.1368 0.178 24.5Hydrogen H2 2.016 0.0695 0.090 13.5Nitrogen N2 28.01 0.967 1.25 14.5Oxygen O2 32.00 1.105 1.43 13.2Source: Reprinted from Lyttle (6). Because of the greater voltage drop across a helium arc than an argon arc,however, higher power inputs and greater sensitivity to variations in the arclength can be obtained with helium. The former allows the welding of thickersections and the use of higher welding speeds. The latter, on the other hand,allows a better control of the arc length during automatic GTAW.1.4.5 Advantages and DisadvantagesGas–tungsten arc welding is suitable for joining thin sections because of itslimited heat inputs. The feeding rate of the ﬁller metal is somewhat indepen-dent of the welding current, thus allowing a variation in the relative amountof the fusion of the base metal and the fusion of the ﬁller metal. Therefore,the control of dilution and energy input to the weld can be achieved withoutchanging the size of the weld. It can also be used to weld butt joints of thinsheets by fusion alone, that is, without the addition of ﬁller metals or autoge-nous welding. Since the GTAW process is a very clean welding process, it canbe used to weld reactive metals, such as titanium and zirconium, aluminum,and magnesium. However, the deposition rate in GTAW is low. Excessive welding currentscan cause melting of the tungsten electrode and results in brittle tungsteninclusions in the weld metal. However, by using preheated ﬁller metals, thedeposition rate can be improved. In the hot-wire GTAW process, the wire isfed into and in contact with the weld pool so that resistance heating can beobtained by passing an electric current through the wire.1.5 PLASMA ARC WELDING1.5.1 The ProcessPlasma arc welding (PAW) is an arc welding process that melts and joins metalsby heating them with a constricted arc established between a tungsten elec-
PLASMA ARC WELDING 17trode and the metals, as shown in Figure 1.14. It is similar to GTAW, but anoriﬁce gas as well as a shielding gas is used. As shown in Figure 1.15, the arc inPAW is constricted or collimated because of the converging action of the oriﬁcegas nozzle, and the arc expands only slightly with increasing arc length (5).Direct-current electrode negative is normally used, but a special variable-polarity PAW machine has been developed for welding aluminum, where thepresence of aluminum oxide ﬁlms prevents a keyhole from being established.1.5.2 Arc InitiationThe tungsten electrode sticks out of the shielding gas nozzle in GTAW (Figure1.11b) while it is recessed in the oriﬁce gas nozzle in PAW (Figure 1.14b). Con-sequently, arc initiation cannot be achieved by striking the electrode tip againstthe workpiece as in GTAW. The control console (Figure 1.14a) allows a pilotarc to be initiated, with the help of a high-frequency generator, between theelectrode tip and the water-cooled oriﬁce gas nozzle. The arc is then gradually Shielding gas (a) Control console Orifice gas Welding direction Power Source Torch Filler rod Cables Workpiece Orifice gas Tungsten Shielding (b) electrode gas Orifice gas nozzle Shielding gas (water cooled) nozzle Orifice Arc plasma Molten metal Weld metal Base metal KeyholeFigure 1.14 Plasma arc welding: (a) overall process; (b) welding area enlarged andshown with keyholing.
18 FUSION WELDING PROCESSES Plasma arc Gas tungsten arcFigure 1.15 Comparison between a gas–tungsten arc and a plasma arc. From WeldingHandbook (5). Courtesy of American Welding Society.transferred from between the electrode tip and the oriﬁce gas nozzle tobetween the electrode tip and the workpiece.1.5.3 KeyholingIn addition to the melt-in mode adopted in conventional arc welding processes(such as GTAW), the keyholing mode can also be used in PAW in certainranges of metal thickness (e.g., 2.5–6.4 mm). With proper combinations of theoriﬁce gas ﬂow, the travel speed, and the welding current, keyholing is possi-ble. Keyholing is a positive indication of full penetration and it allows theuse of signiﬁcantly higher welding speeds than GTAW. For example, it hasbeen reported (7) that PAW took one-ﬁfth to one-tenth as long to completea 2.5-m-long weld in 6.4-mm-thick 410 stainless steel as GTAW. Gas–tungstenarc welding requires multiple passes and is limited in welding speed. As shownin Figure 1.16, 304 stainless steel up to 13 mm (1/2 in.) thick can be welded in asingle pass (8). The wine-cup-shaped weld is common in keyholing PAW.1.5.4 Advantages and DisadvantagesPlasma arc welding has several advantages over GTAW. With a collimated arc,PAW is less sensitive to unintentional arc length variations during manualwelding and thus requires less operator skill than GTAW. The short arc lengthin GTAW can cause a welder to unintentionally touch the weld pool with theelectrode tip and contaminate the weld metal with tungsten. However, PAWdoes not have this problem since the electrode is recessed in the nozzle. Asalready mentioned, the keyhole is a positive indication of full penetration, andit allows higher welding speeds to be used in PAW. However, the PAW torch is more complicated. It requires proper electrodetip conﬁguration and positioning, selection of correct oriﬁce size for the appli-cation, and setting of both oriﬁce and shielding gas ﬂow rates. Because of the
GAS–METAL ARC WELDING 19Figure 1.16 A plasma arc weld made in 13-mm-thick 304 stainless steel with keyhol-ing. From Lesnewich (8).need for a control console, the equipment cost is higher in PAW than in GTAW.The equipment for variable-polarity PAW is much more expensive than thatfor GTAW.1.6 GAS–METAL ARC WELDING1.6.1 The ProcessGas–metal arc welding (GMAW) is a process that melts and joins metals byheating them with an arc established between a continuously fed ﬁller wireelectrode and the metals, as shown in Figure 1.17. Shielding of the arc and themolten weld pool is often obtained by using inert gases such as argon andhelium, and this is why GMAW is also called the metal–inert gas (MIG)welding process. Since noninert gases, particularly CO2, are also used, GMAWseems a more appropriate name. This is the most widely used arc weldingprocess for aluminum alloys. Figure 1.18 shows gas–metal arc welds of 5083aluminum, one made with Ar shielding and the other with 75% He–25% Arshielding (9). Unlike in GTAW, DCEP is used in GMAW. A stable arc, smoothmetal transfer with low spatter loss and good weld penetration can beobtained. With DCEN or AC, however, metal transfer is erratic.1.6.2 Shielding GasesArgon, helium, and their mixtures are used for nonferrous metals as well asstainless and alloy steels. The arc energy is less uniformly dispersed in an Ararc than in a He arc because of the lower thermal conductivity of Ar. Conse-quently, the Ar arc plasma has a very high energy core and an outer mantleof lesser thermal energy. This helps produce a stable, axial transfer of metal
20 FUSION WELDING PROCESSES Flow meter Regulator (a) Wire Wire drive reel & control Welding Wire direction Gun electrode Workpiece Power Shielding Cable 1 Source gas cylinder Cable 2 Wire electrode Shielding gas Contact tube (b) Cable 1 Shielding Shielding gas gas nozzle Metal Arc droplet Weld metal Base metal Weld poolFigure 1.17 Gas–metal arc welding: (a) overall process; (b) welding area enlarged.Figure 1.18 Gas–metal arc welds in 6.4-mm-thick 5083 aluminum made with argon(left) and 75% He–25% Ar (right). Reprinted from Gibbs (9). Courtesy of AmericanWelding Society.droplets through an Ar arc plasma. The resultant weld transverse cross sectionis often characterized by a papillary- (nipple-) type penetration pattern (10)such as that shown in Figure 1.18 (left). With pure He shielding, on the otherhand, a broad, parabolic-type penetration is often observed. With ferrous metals, however, He shielding may produce spatter and Arshielding may cause undercutting at the fusion lines. Adding O2 (about 3%)or CO2 (about 9%) to Ar reduces the problems. Carbon and low-alloy steelsare often welded with CO2 as the shielding gas, the advantages being higher
GAS–METAL ARC WELDING 21welding speed, greater penetration, and lower cost. Since CO2 shielding pro-duces a high level of spatter, a relatively low voltage is used to maintain a shortburied arc to minimize spatter; that is, the electrode tip is actually below theworkpiece surface (10).1.6.3 Modes of Metal TransferThe molten metal at the electrode tip can be transferred to the weld pool bythree basic transfer modes: globular, spray, and short-circuiting.A. Globular Transfer Discrete metal drops close to or larger than theelectrode diameter travel across the arc gap under the inﬂuence of gravity.Figure 1.19a shows globular transfer during GMAW of steel at 180 A andwith Ar–2% O2 shielding (11). Globular transfer often is not smooth andproduces spatter. At relatively low welding current globular transferoccurs regardless of the type of the shielding gas. With CO2 and He, however,it occurs at all usable welding currents. As already mentioned, a shortburied arc is used in CO2-shielded GMAW of carbon and low-alloy steels tominimize spatter.Figure 1.19 Metal transfer during GMAW of steel with Ar–2% O2 shielding: (a)globular transfer at 180 A and 29 V shown at every 3 ¥ 10-3 s; (b) spray transfer at320 A and 29 V shown at every 2.5 ¥ 10-4 s. Reprinted from Jones et al. (11). Courtesyof American Welding Society.
22 FUSION WELDING PROCESSESB. Spray Transfer Above a critical current level, small discrete metal dropstravel across the arc gap under the inﬂuence of the electromagnetic force atmuch higher frequency and speed than in the globular mode. Figure 1.19bshows spray transfer during GMAW of steel at 320 A and with Ar–2% O2shielding (11). Metal transfer is much more stable and spatter free. The criti-cal current level depends on the material and size of the electrode and thecomposition of the shielding gas. In the case of Figure 1.19, the critical currentwas found to be between 280 and 320 A (11).C. Short-Circuiting Transfer The molten metal at the electrode tip is trans-ferred from the electrode to the weld pool when it touches the pool surface,that is, when short circuiting occurs. Short-circuiting transfer encompasses thelowest range of welding currents and electrode diameters. It produces a smalland fast-freezing weld pool that is desirable for welding thin sections, out-of-position welding (such as overhead-position welding), and bridging large rootopenings.1.6.4 Advantages and DisadvantagesLike GTAW, GMAW can be very clean when using an inert shielding gas. Themain advantage of GMAW over GTAW is the much higher deposition rate,which allows thicker workpieces to be welded at higher welding speeds. Thedual-torch and twin-wire processes further increase the deposition rate ofGMAW (12). The skill to maintain a very short and yet stable arc in GTAWis not required. However, GMAW guns can be bulky and difﬁcult-to-reachsmall areas or corners.1.7 FLUX-CORE ARC WELDING1.7.1 The ProcessFlux-core arc welding (FCAW) is similar to GMAW, as shown in Figure 1.20a.However, as shown in Figure 1.20b, the wire electrode is ﬂux cored rather thansolid; that is, the electrode is a metal tube with ﬂux wrapped inside. The func-tions of the ﬂux are similar to those of the electrode covering in SMAW, includ-ing protecting the molten metal from air. The use of additional shielding gasis optional.1.8 SUBMERGED ARC WELDING1.8.1 The ProcessSubmerged arc welding (SAW) is a process that melts and joins metals byheating them with an arc established between a consumable wire electrode
SUBMERGED ARC WELDING 23 Regulator Flow meter (a) Wire Wire drive reel & control Welding Wire direction Gun electrode Power Shielding Workpiece Source gas Cable 1 cylinder Cable 2 Wire electrode Shielding gas Contact tube (b) Cable 1 Shielding gas Metal droplet nozzle Flux droplet Arc Slag Shielding gas (optional) Weld metal Base metal Weld pool Figure 1.20 Flux-core arc welding: (a) overall process; (b) welding area enlarged.and the metals, with the arc being shielded by a molten slag and granular ﬂux,as shown in Figure 1.21. This process differs from the arc welding processesdiscussed so far in that the arc is submerged and thus invisible. The ﬂux is sup-plied from a hopper (Figure 1.21a), which travels with the torch. No shieldinggas is needed because the molten metal is separated from the air by the moltenslag and granular ﬂux (Figure 1.21b). Direct-current electrode positive is mostoften used. However, at very high welding currents (e.g., above 900 A) AC ispreferred in order to minimize arc blow. Arc blow is caused by the electro-magnetic (Lorentz) force as a result of the interaction between the electriccurrent itself and the magnetic ﬁeld it induces.1.8.2 Advantages and DisadvantagesThe protecting and reﬁning action of the slag helps produce clean welds inSAW. Since the arc is submerged, spatter and heat losses to the surroundingair are eliminated even at high welding currents. Both alloying elements andmetal powders can be added to the granular ﬂux to control the weld metalcomposition and increase the deposition rate, respectively. Using two or moreelectrodes in tandem further increases the deposition rate. Because of its high
24 FUSION WELDING PROCESSES Flux hopper Wire reel (a) Wire electrode Wire drive & control Welding Cables direction Power Source Workpiece Granular flux Droplet Wire electrode Arc Molten slag (b) Solidified slag Base metal Weld metal Metal poolFigure 1.21 Submerged arc welding: (a) overall process; (b) welding area enlarged.deposition rate, workpieces much thicker than that in GTAW and GMAW canbe welded by SAW. However, the relatively large volumes of molten slag andmetal pool often limit SAW to ﬂat-position welding and circumferentialwelding (of pipes). The relatively high heat input can reduce the weld qualityand increase distortions.1.9 ELECTROSLAG WELDING1.9.1 The ProcessElectroslag welding (ESW) is a process that melts and joins metals by heatingthem with a pool of molten slag held between the metals and continuouslyfeeding a ﬁller wire electrode into it, as shown in Figure 1.22. The weld poolis covered with molten slag and moves upward as welding progresses. A pairof water-cooled copper shoes, one in the front of the workpiece and onebehind it, keeps the weld pool and the molten slag from breaking out. Similarto SAW, the molten slag in ESW protects the weld metal from air and reﬁnesit. Strictly speaking, however, ESW is not an arc welding process, because thearc exists only during the initiation period of the process, that is, when the arc
ELECTROSLAG WELDING 25 Wire reel Wire feed motor & control Workpiece Cable Water- cooled Power (a) Source copper shoes Cable Bottom support Wire electrode Consumable guide tube Base metal (b) Molten slag Weld pool Weld metal Figure 1.22 Electroslag welding: (a) overall process; (b) welding area enlarged.heats up the ﬂux and melts it. The arc is then extinguished, and the resistanceheating generated by the electric current passing through the slag keeps itmolten. In order to make heating more uniform, the electrode is often oscil-lated, especially when welding thicker sections. Figure 1.23 is the transversecross section of an electroslag weld in a steel 7 cm thick (13). Typical examplesof the application of ESW include the welding of ship hulls, storage tanks, andbridges.1.9.2 Advantages and DisadvantagesElectroslag welding can have extremely high deposition rates, but only onesingle pass is required no matter how thick the workpiece is. Unlike SAW orother arc welding processes, there is no angular distortion in ESW because the
26 FUSION WELDING PROCESSESFigure 1.23 Transverse cross section of electroslag weld in 70-mm-thick steel.Reprinted from Eichhorn et al. (13). Courtesy of American Welding Society. Deposition Rate, Lb/hr 0 40 80 120 160 200 6010 6012 SMAW Welding Process (100% Duty Cycle) 7018 7024 cold GTAW/PAW wire fine wire spray GMAW CO2 shielded FCAW iron powder SAW with iron powder added 1 electrode 2 electrodes 3 electrodes ESW 4 electrodes 5 electrodes 0 20 40 60 80 Deposition Rate, Kg/hr Figure 1.24 Deposition rate in arc welding processes. Modiﬁed from Cary (14).weld is symmetrical with respect to its axis. However, the heat input is veryhigh and the weld quality can be rather poor, including low toughness causedby the coarse grains in the fusion zone and the heat-affected zone. Electroslagwelding is restricted to vertical position welding because of the very largepools of the molten metal and slag. Figure 1.24 summarizes the deposition rates of the arc welding processesdiscussed so far (14). As shown, the deposition rate increases in the order of
ELECTRON BEAM WELDING 27GTAW, SMAW, GMAW and FCAW, SAW, and ESW. The deposition rate canbe much increased by adding iron powder in SAW or using more than onewire in SAW, ESW, and GMAW (not shown).1.10 ELECTRON BEAM WELDING1.10.1 The ProcessElectron beam welding (EBW) is a process that melts and joins metals byheating them with an electron beam. As shown in Figure 1.25a, the cathode ofthe electron beam gun is a negatively charged ﬁlament (15). When heated upto its thermionic emission temperature, this ﬁlament emits electrons. Theseelectrons are accelerated by the electric ﬁeld between a negatively chargedbias electrode (located slightly below the cathode) and the anode. They passthrough the hole in the anode and are focused by an electromagnetic coil toa point at the workpiece surface. The beam currents and the acceleratingvoltages employed for typical EBW vary over the ranges of 50–1000 mA and30–175 kV, respectively. An electron beam of very high intensity can vaporizethe metal and form a vapor hole during welding, that is, a keyhole, as depictedin Figure 1.25b. Figure 1.26 shows that the beam diameter decreases with decreasingambient pressure (1). Electrons are scattered when they hit air molecules, andthe lower the ambient pressure, the less they are scattered. This is the mainreason for EBW in a vacuum chamber. The electron beam can be focused to diameters in the range of 0.3–0.8 mmand the resulting power density can be as high as 1010 W/m2 (1). The very high bias high electrode voltage cathode electron anode beam focusing weld coil weldingn weld pool bead directio vacuum chamber electron moten beam metal to cross- keyhole section pump specimen of weld (a) (b)Figure 1.25 Electron beam welding: (a) process; (b) keyhole. Modiﬁed from Arata(15).
28 FUSION WELDING PROCESSES 750 torr 500 torr 250 torr 50 torr 5 torrFigure 1.26 Dispersion of electron beam at various ambient pressures (1). Reprintedfrom Welding Handbook (1). Courtesy of American Welding Society. gas tungsten arc weld electron beam 13 mm weld (0.5 in) (a) (b)Figure 1.27 Welds in 13-mm-thick 2219 aluminum: (a) electron beam weld; (b)gas–tungsten arc weld. From Farrell (16).power density makes it possible to vaporize the material and produce a deep-penetrating keyhole and hence weld. Figure 1.27 shows a single-pass electronbeam weld and a dual-pass gas–tungsten arc weld in a 13-mm-thick (0.5-in.)2219 aluminum, the former being much narrower (16). The energy requiredper unit length of the weld is much lower in the electron beam weld (1.5 kJ/cm,or 3.8 kJ/in.) than in the gas–tungsten arc weld (22.7 kJ/cm, or 57.6 kJ/in.). Electron beam welding is not intended for incompletely degassed materi-als such as rimmed steels. Under high welding speeds gas bubbles that do nothave enough time to leave deep weld pools result in weld porosity. Materialscontaining high-vapor-pressure constituents, such as Mg alloys and Pb-containing alloys, are not recommended for EBW because evaporation ofthese elements tends to foul the pumps or contaminate the vacuum system.1.10.2 Advantages and DisadvantagesWith a very high power density in EBW, full-penetration keyholing is possi-ble even in thick workpieces. Joints that require multiple-pass arc welding can
LASER BEAM WELDING 29 SB49 A387 Missed joint (a) 48356 47421 (b)Figure 1.28 Missed joints in electron beam welds in 150-mm-thick steels: (a)2.25Cr–1Mo steel with a transverse ﬂux density of 3.5 G parallel to joint plane; (b) SB(C–Mn) steel and A387 (2.25Cr–1Mo) steel. Reprinted from Blakeley and Sanderson(17). Courtesy of American Welding Society.be welded in a single pass at a high welding speed. Consequently, the totalheat input per unit length of the weld is much lower than that in arc welding,resulting in a very narrow heat-affected zone and little distortion. Reactiveand refractory metals can be welded in vacuum where there is no air to causecontamination. Some dissimilar metals can also be welded because the veryrapid cooling in EBW can prevent the formation of coarse, brittle intermetal-lic compounds. When welding parts varying greatly in mass and size, the abilityof the electron beam to precisely locate the weld and form a favorably shapedfusion zone helps prevent excessive melting of the smaller part. However, the equipment cost for EBW is very high. The requirement ofhigh vacuum (10-3–10-6 torr) and x-ray shielding is inconvenient and time con-suming. For this reason, medium-vacuum (10-3–25 torr) EBW and nonvacuum(1 atm) EBW have also been developed. The ﬁne beam size requires preciseﬁt-up of the joint and alignment of the joint with the gun. As shown in Figure1.28, residual and dissimilar metal magnetism can cause beam deﬂection andresult in missed joints (17).1.11 LASER BEAM WELDING1.11.1 The ProcessLaser beam welding (LBW) is a process that melts and joins metals by heatingthem with a laser beam. The laser beam can be produced either by a solid-
30 FUSION WELDING PROCESSESstate laser or a gas laser. In either case, the laser beam can be focused anddirected by optical means to achieve high power densities. In a solid-statelaser, a single crystal is doped with small concentrations of transition elementsor rare earth elements. For instance, in a YAG laser the crystal of yttrium–aluminum–garnet (YAG) is doped with neodymium. The electrons of thedopant element can be selectively excited to higher energy levels upon expo-sure to high-intensity ﬂash lamps, as shown in Figure 1.29a. Lasing occurs whenthese excited electrons return to their normal energy state, as shown in Figure1.29b. The power level of solid-state lasers has improved signiﬁcantly, and con-tinuous YAG lasers of 3 or even 5 kW have been developed. In a CO2 laser, a gas mixture of CO2, N2, and He is continuously excitedby electrodes connected to the power supply and lases continuously. Higher Reflecting mirror Power source Crystal High (a) intensity flash lamp Cooling system Patially reflecting mirror Focusing lens Pool Weld Travel direction Workpiece energy absorbed energy emitted from flash lamp as heat excited outer intermediate electron energy ground levels inner electrons nucleus (b) energy normal emitted as electron light (photon) orbitsFigure 1.29 Laser beam welding with solid-state laser: (a) process; (b) energy absorp-tion and emission during laser action. Modiﬁed from Welding Handbook (1).
LASER BEAM WELDING 31 laser beam weldingn weld pool weld directio bead molten metal cross- keyhole section of weld 2 mm (a) (b)Figure 1.30 Laser beam welding with CO2 laser: (a) process; (b) weld in 13-mm-thickA633 steel. (b) Courtesy of E.A. Metzbower.power can be achieved by a CO2 laser than a solid-state laser, for instance,15 kW. Figure 1.30a shows LBW in the keyholing mode. Figure 1.30b shows aweld in a 13-mm-thick A633 steel made with a 15-kW CO2 laser at 20 mm/s(18). Besides solid-state and gas lasers, semiconductor-based diode lasers havealso been developed. Diode lasers of 2.5 kW power and 1 mm focus diameterhave been demonstrated (19). While keyholing is not yet possible, conduction-mode (surface melting) welding has produced full-penetration welds with adepth–width ratio of 3 : 1 or better in 3-mm-thick sheets.1.11.2 ReﬂectivityThe very high reﬂectivity of a laser beam by the metal surface is a well-knownproblem in LBW. As much as about 95% of the CO2 beam power can bereﬂected by a polished metal surface. Reﬂectivity is slightly lower with a YAGlaser beam. Surface modiﬁcations such as roughening, oxidizing, and coatingcan reduce reﬂectivity signiﬁcantly (20). Once keyholing is established, absorp-tion is high because the beam is trapped inside the hole by internal reﬂection.1.11.3 Shielding GasA plasma (an ionic gas) is produced during LBW, especially at high powerlevels, due to ionization by the laser beam. The plasma can absorb and scatterthe laser beam and reduce the depth of penetration signiﬁcantly. It is there-fore necessary to remove or suppress the plasma (21). The shielding gas forprotecting the molten metal can be directed sideways to blow and deﬂect theplasma away from the beam path. Helium is often preferred to argon as theshielding gas for high-power LBW because of greater penetration depth (22).
32 FUSION WELDING PROCESSESSince the ionization energy of helium (24.5 eV) is higher than that of argon(15.7 eV), helium is less likely to be ionized and become part of the plasmathan argon. However, helium is lighter than air and is thus less effective in dis-placing air from the beam path. Helium–10% Ar shielding has been foundto improve penetration over pure He at high-speed welding where a lightshielding gas may not have enough time to displace air from the beam path(23).1.11.4 Lasers in Arc WeldingAs shown in Figure 1.31, laser-assisted gas metal arc welding (LAGMAW) hasdemonstrated signiﬁcantly greater penetration than conventional GMAW(24). In addition to direct heating, the laser beam acts to focus the arc byheating its path through the arc. This increases ionization and hence the con-ductivity of the arc along the beam path and helps focus the arc energy alongthe path. It has been suggested that combining the arc power with a 5-kW CO2laser, LAGMAW has the potential to achieve weld penetration in mild steelequivalent to that of a 20–25-kW laser (24). Albright et al. (25) have shownthat a lower power CO (not CO2) laser of 7 W and 1 mm diameter can initi-ate, guide, and focus an Ar–1% CO gas–tungsten arc.1.11.5 Advantages and DisadvantagesLike EBW, LBW can produce deep and narrow welds at high welding speeds,with a narrow heat-affected zone and little distortion of the workpiece. It can 12 10 Penetration (mm) 8 6 4 LAGMAW 2 GMAW 0 300 400 500 600 700 Welding current (A)Figure 1.31 Weld penetration in GMAW and laser-assisted GMAW using CO2 laserat 5.7 kW. Reprinted from Hyatt et al. (24). Courtesy of American Welding Society.
REFERENCES 33be used for welding dissimilar metals or parts varying greatly in mass and size.Unlike EBW, however, vacuum and x-ray shielding are not required in LBW.However, the very high reﬂectivity of a laser beam by the metal surface is amajor drawback, as already mentioned. Like EBW, the equipment cost is veryhigh, and precise joint ﬁt-up and alignment are required.REFERENCES 1. Welding Handbook, Vol. 3, 7th ed., American Welding Society, Miami, FL, 1980, pp. 170–238. 2. Mendez, P. F., and Eagar, T. W., Advanced Materials and Processes, 159: 39, 2001. 3. Welding Handbook, Vol. 1, 7th ed., American Welding Society, Miami, FL, 1976, pp. 2–32. 4. Welding Workbook, Data Sheet 212a, Weld. J., 77: 65, 1998. 5. Welding Handbook, Vol. 2, 7th ed., American Welding Society, Miami, FL, 1978, pp. 78–112, 296–330. 6. Lyttle, K. A., in ASM Handbook, Vol. 6, ASM International, Materials Park, OH, 1993, p. 64. 7. Schwartz, M. M., Metals Joining Manual, McGraw-Hill, New York, 1979, pp. 2–1 to 3– 40. 8. Lesnewich, A., in Weldability of Steels, 3rd ed., Eds. R. D. Stout and W. D. Doty, Welding Research Council, New York, 1978, p. 5. 9. Gibbs, F. E., Weld. J., 59: 23, 1980.10. Fact Sheet—Choosing Shielding for GMA Welding, Weld. J., 79: 18, 2000.11. Jones, L. A., Eagar, T. W., and Lang, J. H., Weld. J., 77: 135s, 1998.12. Blackman, S. A., and Dorling, D. V., Weld. J., 79: 39, 2000.13. Eichhorn, F., Remmel, J., and Wubbels, B., Weld. J., 63: 37, 1984.14. Cary, H. B., Modern Welding Technology, Prentice-Hall, Englewood Cliffs, NJ, 1979.15. Arata, Y., Development of Ultra High Energy Density Heat Source and Its Appli- cation to Heat Processing, Okada Memorial Japan Society, 1985.16. Farrell, W. J., The Use of Electron Beam to Fabricate Structural Members, Creative Manufacturing Seminars, ASTME Paper SP 63-208, 1962–1963.17. Blakeley, P. J., and Sanderson, A., Weld. J., 63: 42, 1984.18. Metzbower, E. A., private communication, Naval Research Laboratory, Washington, DC.19. Bliedtner, J., Heyse, Th., Jahn, D., Michel, G., Muller, H., and Wolff, D., Weld. J., 80: 47, 2001.20. Xie, J., and Kar, A., Weld. J., 78: 343s, 1999.21. Mazumder, J., in ASM Handbook, Vol. 6, ASM International, Materials Park, OH, 1993, p. 874.22. Rockstroh, T., and Mazumder, J., J. Appl. Phys., 61: 917, 1987.
34 FUSION WELDING PROCESSES23. Seaman, F., Role of Shielding Gas in Laser Welding, Technical Paper MR77-982, Society of Manufacturing Engineers, Dearborn, MI, 1977.24. Hyatt, C. V., Magee, K. H., Porter, J. F., Merchant, V. E., and Matthews, J. R., Weld. J., 80: 163s, 2001.25. Albright, C. E., Eastman, J., and Lempert, W., Weld. J., 80: 55, 2001.26. Ushio, M., Matsuda, F., and Sadek, A. A., in “ International Trends in Welding Science and Technology, Eds. S. A. David and J. M. Vitek, ASM International, Materials Park, OH, March 1993, p. 408.FURTHER READING1. Arata, Y., Development of Ultra High Energy Density Heat Source and Its Applica- tion to Heat Processing, Okada Memorial Society for the Promotion of Welding, Japan, 1985.2. Schwartz, M. M., Metals Joining Manual, McGraw-Hill, New York, 1979.3. Welding Handbook, Vols. 1–3, 7th ed., American Welding Society, Miami, FL, 1980.4. Duley, W. W., Laser Welding, Wiley, New York, 1999.5. ASM Handbook, Vol. 6, ASM International, Materials Park, OH, 1993.PROBLEMS1.1 It has been suggested that compared to SMAW, the cooling rate is higher in GMAW and it is, therefore, more likely for heat-affected zone cracking to occur in hardenable steels. What is the main reason for the cooling rate to be higher in GMAW than SMAW?1.2 The diameter of the electrodes to be used in SMAW depends on factors such as the workpiece thickness, the welding position, and the joint design. Large electrodes, with their corresponding high currents, tend to produce large weld pools. When welding in the overhead or vertical position, do you prefer using larger or smaller electrodes?1.3 In arc welding, the magnetic ﬁeld induced by the welding current passing through the electrode and the workpiece can interact with the arc and cause “arc blow.” Severe arc blow can cause excessive weld spatter and incomplete fusion. When arc blow is a problem in SMAW, do you expect to minimize it by using DC or AC for welding?1.4 In the hot-wire GTAW process, shown in Figure P1.4, the tip of the ﬁller metal wire is dipped in the weld pool and the wire itself is resistance heated by means of a second power source between the contact tube of the wire and the workpiece. In the case of steels, the deposition rate can
PROBLEMS 35 Filler wire Tungsten electrode Wire feeder Contact tube Contact tube Cable 1 Shielding gas nozzle 2nd Cable 3 Arc Shielding gas power source Cable 4 Weld metal Base metal Weld pool Figure P1.4 be more than doubled this way. Do you prefer using an AC or a DC power source for heating the wire? Do you expect to apply this process to aluminum and copper alloys?1.5 In GTAW the welding cable is connected to the tungsten electrode through a water-cooled copper contact tube, as shown in Figure 1.11. Why is the tube positioned near the lower end of the electrode instead of the top?1.6 Measurements of the axial temperature distribution along the GTAW electrode have shown that the temperature drops sharply from the electrode tip toward the contact tube. Why? For instance, with a 2.4-mm-diameter W–ThO2 electrode at 150 A, the temperature drops from about 3600 K at the tip to about 2000 K at 5 mm above the tip. Under the same condition but with a W–CeO2 electrode, the tempera- ture drops from about 2700 K at the tip to about 1800 K at 5 mm above the tip (26). Which electrode can carry more current before melting and why?1.7 Experimental results show that in EBW the penetration depth of the weld decreases as the welding speed increases. Explain why. Under the same power and welding speed, do you expect a much greater penetra- tion depth in aluminum or steel and why?1.8 How does the working distance in EBW affect the depth–width ratio of the resultant weld?1.9 Consider EBW in the presence of a gas environment. Under the same power and welding speed, rank and explain the weld penetration for Ar, He, and air. The speciﬁc gravities of Ar, He, and air with respect to air are 1.38, 0.137, and 1, respectively, at 1 atm, 0°C.
36 FUSION WELDING PROCESSES weld transverse cross-section 1 mm 1 mm Figure P1.10 steel 15 cm weld steel transverse cross-section 15 cm Figure P1.111.10 Which arc welding process could have been used for joining the edge weld of thin-gauge steel shown in Figure P1.10 and why?1.11 Two 15-cm-thick steel plates were joined together in a single pass, as shown in Figure P1.11. Which welding process could have been used and why?
Welding Metallurgy, Second Edition. Sindo Kou Copyright 2003 John Wiley & Sons, Inc. ISBN: 0-471-43491-42 Heat Flow in WeldingHeat ﬂow during welding, as will be shown throughout Parts II–IV of thisbook, can strongly affect phase transformations during welding and thus theresultant microstructure and properties of the weld. It is also responsible forweld residual stresses and distortion, as will be discussed in Chapter 5.2.1 HEAT SOURCE2.1.1 Heat Source EfﬁciencyA. Deﬁnition The heat source efﬁciency h is deﬁned as Qt weld Q h= = (2.1) Qnominalt weld Qnominalwhere Q is the rate of heat transfer from the heat source to the workpiece,Qnominal the nominal power of the heat source, and tweld the welding time. Aportion of the power provided by the heat source is transferred to the work-piece and the remaining portion is lost to the surroundings. Consequently,h < 1. If the heat source efﬁciency h is known, the heat transfer rate to theworkpiece, Q, can be easily determined from Equation (2.1). In arc welding with a constant voltage E and a constant current I, the arcefﬁciency can be expressed as Qt weld Q h= = (2.2) EIt weld EIEquation (2.2) can also be applied to electron beam welding, where h is theheat source efﬁciency. In laser beam welding, Qnominal in Equation (2.1) is thepower of the laser beam, for instance, 2500 W. It should be noted that in the welding community the term heat input oftenrefers to Qnominal, or EI in the case of arc welding, and the term heat input perunit length of weld often refers to the ratio Qnominal/V, or EI/V, where V is thewelding speed.B. Measurements The heat source efﬁciency can be measured with acalorimeter. The heat transferred from the heat source to the workpiece is in 37
38 HEAT FLOW IN WELDING GTAW Pipe torch Arc Water in Water out Thermocouple Insulation Thermocouple (a) Temperature, oF 50 Shaded area 120 Temperature, oC ∞ =∫ [ ]dt 40 0 Tout- Tin 100 Tout 30 80 Tin 20 100 120 Time, seconds (b)Figure 2.1 Measurement of arc efﬁciency in GTAW: (a) calorimeter; (b) rise in coolingwater temperature as a function of time. Modiﬁed from Kou et al. (1, 2).turn transferred from the workpiece to the calorimeter, which can be deter-mined as described below. Kou et al. (1, 2) used simple tubular calorimeters to determine the arcefﬁciency in GTAW of aluminum, as shown in Figure 2.1a. The calorimetercan be a round cross section if the workpiece is a pipe or a rectangularcross section if the workpiece is a sheet. The temperature rise in the cool-ing water (Tout - Tin) can be measured using thermocouples or thermistors.Heat transfer from the workpiece to the calorimeter is as follows (1–3): • • Qt weld = Ú0 WC (Tout - Tin ) dt ª WC Ú0 (Tout - Tin )dt (2.3)where W is the mass ﬂow rate of water, C the speciﬁc heat of water, Tout theoutlet water temperature, Tin the inlet water temperature, and t time. The inte-gral corresponds to the shaded area in Figure 2.1b. The arc efﬁciency h can bedetermined from Equations (2.2) and (2.3). Giedt et al. (4) used the Seebeck envelop calorimeter shown in Figure 2.2ato measure the arc efﬁciency in GTAW. The name Seebeck came fromthe Seebeck thermoelectric effect of a thermocouple, namely, a voltage isproduced between two thermocouple junctions of different temperatures.The torch can be quickly withdrawn after welding, and the calorimeter lidcan be closed to minimize heat losses to the surrounding air. As shown inFigure 2.2b, heat transfer from the workpiece to the calorimeter can bedetermined by measuring the temperature difference DT and hence gradient